Advantages and disadvantages of the main routes of administration.
In recent years, the development of various cyclodextrin (CD)-based nanosponges (NSs) has gained great importance in the controlled and-or targeted release of drugs due to their versatility and simple preparation. In this chapter, an introduction of different administration routes is explained. Further, different ways to obtain CD-NSs and their classification are shown with a brief explanation of the characterization of the inclusion complexes. Finally, illustrative examples in diverse processes or diseases will be reviewed and explained to demonstrate the potential of CD-NSs. Therefore, this division will serve to compile information on CD-NSs in recent years and to illustrate to readers how to generate and apply different derivatives of interest.
- Cyclodextrin nanosponges
- drug delivery
Society demands better treatments for each disease and therefore the industry tries to obtain them. Novel drugs with better bioactivity are researched to achieve the best result in our bodies. However, several novel drugs present problems related to their chemical properties that prevent them from being used as a pharma or nutraceutical product. The molecule can be unstable in water solution, and/or easily oxidized, and presents poor bioavailability. Different strategies might improve the current therapy. One possibility is to find a good formulation, which stabilizes the drug or carries it to the desired tissue. Moreover, the adverse effect due to the dosage can also be reduced. For this reason, a great number of carriers are been proposed to challenge the previous problems.
One of them is called cyclodextrin (CD), truncated cone-shaped oligosaccharides made up of α-(1→4) linked glucopyranoside units with six, seven and eight glucose units, α, β and γ-CD, respectively [1, 2]. A derivative called 2-Hydroxypropyl-βCD (HPβ-CD) is used as an orphan drug for Niemann Pick disease type C [3, 4]. Complexes formed of molecules and cyclodextrins (CDs) are called “inclusion complexes”. Generally, CDs encapsulate poorly water-soluble compounds and hydrophobic moieties of amphiphilic molecules. Nevertheless, the solubility of these complexes not only depends on the CD used but also on different factors such as pH or guess molecule [5, 6, 7, 8]. The capacity of CDs to increase solubility and protect several molecules has increased their use in the pharmaceutical and food industries [1, 9, 10].
However, the improvement achieved by adding CDs is sometimes insufficient. Then, researchers developed a novel material based on these excipients baptized as Cyclodextrin-based Nanosponge (CD-NS), innovative cross-linked polymer structures with a three-dimensional network, and with a crystalline and amorphous structure, spherical and possessing good swelling properties . Recent reviews [12, 13, 14] point to their wide potential and minimal toxicity [15, 16]. Some applications of these polymers include i) increasing the apparent solubility of poorly soluble drugs, ii) modulating drug release and activity, iii) protecting drugs against several agents, iv) enhancing bioactivities, v) absorbing contaminants ability, vi) delivering the drug, etc.
Cross-linking CDs brings significant benefits to CD-NSs compared with the respective native CDs. In general, CD-NSs can form complexes with a series of different molecules due to their structure. They achieve a hindered diffusion of loaded guest molecules, thus promoting slower release kinetics [17, 18]. Another important property of CD-NSs is that they can be easily recovered from aqueous media and recycled. Although they are insoluble, soluble hyperbranched NS can also be synthesized . Finally, one of their principal disadvantages has been recently solved, they have been tested as a good carrier not only for small molecules but also for higher ones like proteins [20, 21].
This chapter tends to be a first step for the researcher who starts with CD-NSs: i) an introduction of the routes of administration, including advantages and disadvantages is explained, ii) an explanation about the various types of CD-NSs, including its synthesis and classification is written, iii) the different ways to characterize the inclusion complexes are reported and iv) examples of smart delivery are displayed as an encourage study to demonstrate their potential.
2. Routes of administration, advantages, and disadvantages
The choice of the route of administration is crucial as it dramatically affects drug bioavailability and thus requires specific delivery strategies. Parenteral routes include intravenous, intramuscular, and subcutaneous routes, whereas the enteral routes are the oral, sublingual, and rectal routes . Others are inhalation, intranasal, etc. . In this section, each route will be described briefly and special attention will be paid to the oral route, which is the most desired but, at the same time, the most challenging.
When administered via intravenous injection (IV), the drug reaches the systemic circulation directly bypassing absorption and carrying out its effect rapidly. This route is ideal for unstable or scarcely absorbed drugs (e.g. blood products), and irritating drug formulations, the administration of which via subcutaneous and intramuscular routes will be painful. It is also intended for patients who are not able to take the formulations orally, due to mental disorders, nausea, or vomiting.
Intramuscular injection (IM) can involve various muscles, including the gluteal muscle to which up to 5 ml of the formulation can be administered. Via this route, aqueous or oil-based solutions, suspensions, and emulsions are accepted. Aqueous solutions are generally absorbed in 10–30 minutes, whereas drugs insoluble at interstitial pH or suspended in oil-based solutions present a long time of absorption. Vascularisation of the muscle, the volume, and the osmolarity of the injected formulations also affect the absorption time. A depot preparation of the drug can be given via this route with a sustained release of the drug into the bloodstream. IM injection is selected when the drug has a low oral bioavailability or when the patient is not compliant. Vaccines are also administered via this route.
Subcutaneous injections can be given in the forearm or abdomen. Up to 2 ml of the formulation can be administered. Together with aqueous solutions and suspensions, adrenalin can be added to induce vasoconstriction and therefore increase the residence time of drugs (e.g. local anesthetics) or hyaluronidase to make the extracellular matrix more fluid, thus improving the absorption rate.
The absorption rate is extremely variable as it is influenced by the blood flow. Subcutaneous injections are also used for depot formulations. It is easy to administer and requires minimal skills, thus allowing self-administration. Insulin and heparin are given via this route.
Among all, oral delivery has been recognized as the most attractive route, as it is cheap, simple, accepted by patients, requires fewer sterility restrictions, and offers more possibilities in the design of the formulation (including sustained and controlled delivery) . It is used for drugs with topical action in the gut and systemic effects when they reach the bloodstream. However, it is not suitable for emergencies in which an immediate effect is fundamental.
Over the past few years, many efforts have been made to develop oral delivery systems able to overcome the obstacles in the gastrointestinal tract (GI) in which the mechanism of absorption is complex with multiple levels of barriers .
There is a long list of variables that influence the GI absorption of drugs, which are grouped in technical challenges, physicochemical properties of the drug, and environmental factors .
The technical challenges concern the pharmaceutical form, i.e. liquid or solid. In solid forms,
Most drugs are absorbed in the small intestine, characterized by a large surface area of absorption and having a crucial influence on bioavailability.
The walls of the GI tract are characterized by the presence of mucus, which has been a target for drug delivery systems (DDS) capable of mucopenetration or mucoadhesion . Mucopenetration consists in regulating the hydrophobicity/hydrophilicity of the carrier’s matrix or combining mucolytic enzymes to promote drug penetration. On the contrary, mucoadhesive carriers, which have attracted significant attention [26, 27, 28], can adhere to mucus, thus increasing the residence time. CD NSs have proven to possess this property, making them particularly promising for oral delivery .
Last but not least, the first-pass effect should be borne in mind when dealing with the oral route as it is certainly a limiting factor. It refers to the metabolism (mainly in the liver) of the drug before it reaches the systemic circulation, which may lead to a drop in bioavailability . For this reason, several drugs are administered via other enteral routes (e.g. rectal and sublingual).
The sublingual route offers the benefit of bypassing the first-pass effect due to the passive diffusion through the highly permeable mucosa underneath the tongue. It is simple with a low risk of infection and the effect is rapid. Nitroglycerin is administered via this route.
The rectal route exploits the highly vascularized rectal mucosa for drug absorption. The first-pass effect is partially avoided. It is indicated for patients with gastrointestinal motility problems, nausea, vomiting, and children.
Inhalation is used to obtain a rapid effect as the drug crosses the large surface area of the respiratory tract epithelium and reaches the systemic circulation. It avoids the first-pass metabolism. The particle size and morphology of the formulation inhaled are crucial. It is mainly used for the treatment of respiratory diseases. The intranasal route enables the drug to be absorbed via passive diffusion across the highly-vascularised respiratory epithelium directly into the systemic circulation. Nasal decongestants and anti-allergic drugs are administered via this route (Table 1).
|Route of administration||Advantages||Disadvantages|
3. Synthesis and classification of CD-NSs
The choice of appropriate synthetic conditions, allowed to obtain both water-soluble and water-insoluble polymer products, known also as CD-NSs or insoluble, and branched or soluble polymer [30, 31, 32]. The latter case allowed to overcome the limits of pristine CDs in terms of solubility in water and specific organic solvent, while the resulting formation of a three-dimensional cross-linked network was related to the presence of interstitial spaces among the monomers . In this regard, the nature of the cross-linker and its amount in respect to the CD, ratio which defines the so-called cross-linking density, are presented to have a great impact on the properties and structure of the final material . Also, being said interstices wider and more hydrophilic in respect to the cavities of CDs, a wider hosting capability was observed as a result.
3.1 General synthesis protocol
The most common method announced for the synthesis of CD based polymers, is characterized by employing a suitable solvent which could be either organic solvent or, in specific cases water, for the dissolution of the CDs. Afterwards, under continuous stirring, the chosen linking agent is added to the solution. Nevertheless, when required, the introduction of a catalyst occurs before the linking agent, and in specific cases, an increase in temperature is necessary to start the cross-linking reactions. The use of an ultrasound bath instead of stirring was also considered . Eventually, either a sol–gel process or a precipitation polymerization can be observed, leading to the formation of a monolithic block or a precipitate, respectively. Also, in those cases in which the cross-linker is in the liquid form, and able to solubilize the CD, a melt polymerization can be performed [36, 37].
Once the synthesis is completed, the solvent, the catalyst, eventual unreacted monomers, and by-products are removed from the synthesized product by purification with water or other volatile solvents. In the end, a dry solid powder is collected [37, 38, 39]. Another well-known approach to synthesize CD-NSs is achieved through simple dehydration reactions. In this case, the CDs and the cross-linker, which is usually an acid bearing two or more carboxylic groups, are solubilized in water. After the addition of a suitable catalyst, the solution is heated to remove the water introduced as solvent as well as the water released as a by-product of the cross-linking condensation reaction. Moreover, the use of vacuum together with the temperature allows to shift the equilibrium of the reaction toward the products [40, 41]. Besides, less used synthetic routes report the use of interfacial or radical polymerization. In the first case, two immiscible phases such as a water solution of CD and a chlorinated solvent solution containing the chosen cross-linker, are mixed and stirred vigorously. The cross-linking occurs rapidly at the interface of the immiscible phases, and a precipitate is obtained . While in the second case, a multistep procedure involving also preliminary derivatization of CD was displayed .
3.2 General classification
In general, based on the technological evolution of these materials, CD-NSs can be classified into four generations, considering their chemical composition and properties . The first generation comprises all those NSs synthesized by a simple one-step reaction of CDs with a cross-linker. This generation was further divided into sub-categories according to the chemical nature of the linking molecules adopted for the synthesis. In this frame, carbonate, ester, ether, and urethane types are the most reported. These specific types of NSs will be described in more detail in the following paragraphs. Subsequently, the introduction of specific functions such as charge or luminescence to the final polymer structure defined the second generation of NSs. These materials displayed more complex polymer architectures achieved either via pre- or post-synthesis functionalization. In the first case, the introduced functions were limited to the surface of the polymer, whereas in the second case a more homogeneous distribution was observed. Referring to the division into generations, the 3rd generation deals with stimuli-responsive NSs, able to modulate their behavior (for example increasing/decreasing a drug release) according to the external environment.
3.2.1 CD-based polyurethane NSs
Urethane, or carbamate, CD-NSs are synthesized by reacting CDs (or a different dextrin) with a suitable diisocyanate as, for example, hexamethylene diisocyanate (HDI), toluene–2,4-diisocyanate (TDI). The reaction scheme is reported below (Figure 1, inset a). The resulting NSs are usually characterized by a rigid structure and a negligible swelling in water (in comparison with other CD-NSs), and organic solvent and high resistance to chemical degradation. Carbamate CD-NSs, were originally developed by Li and Ma for the treatment of wastewaters, as an alternative for activated carbon. They demonstrated with NSs remarkable performances in the removal of organic molecules such as p-nitrophenol reducing concentration of waste from 10−7–10−9 M to ppt level. The surface area was usually lower than activated carbon, (1–2 m2/g, two orders of magnitude) but it is supposed that organic molecules can be adsorbed, diffuse through the surface, and be absorbed inside the bulk of NSs .
The good affinity of organic molecules showed for pollutants , is also demonstrated by the application of urethane NSs in the complexation with biologically relevant compounds, such as bilirubin or amino acids. In 2006, Tang et al. evaluated the difference in absorption of aromatic amino acids and branched-chain amino acids: the absorption of branched-chain amino acids was negligible whereas NSs absorbed 24% of the aromatic amino acids.
In previous works the same polymer was tested for the absorption of bilirubin, reducing the initial concentration of bilirubin (40 mg/l) up to 92.6% after the addition of the NS .
3.2.2 CD-based polycarbonate NSs
Polycarbonate CD-NSs are usually synthesized using active difunctional carbonyl compounds such as 1,1′-carbonyldiimidazole, triphosgene, and diphenylcarbonate (Figure 1, inset b). Since the resulting CD NSs present carbonate bonds between CD monomers, these NSs present short cross-linking bridges and, consequentially, a reduced swelling ability (if compared to CD- based polyesters NSs, for example) and good stability to acidic solutions. The affinity to organic molecules and the surface area are comparable to carbamate NS . The ability of β-CD carbonate NS to remove from wastewater chlorinated persistent organic pollutants (also known as POP) was investigated by Trotta and Cavalli in 2009 : the absorption efficiency was higher than the average of activated carbon. For the specific case of hexachlorobenzene the NS was capable of removing around 99.5% of the pollutant.
An interesting method to evaluate the degree of cross-linking of carbonate β-CD NSs, employing infrared and Raman spectroscopy, was described by Castiglione et al. . Data from spectroscopic analysis and chemical computation demonstrated a correlation between the intensity of carbonyl absorption peak and the degree of cross-linking: the degree of cross-linking increased with the amount of cross-linker, in total agreement with the stoichiometry. Dealing with sugar-based predominantly amorphous materials, the reported method represents a valid and advantageous alternative to x-ray. The crosslinking density or the amount of crosslinker, strongly influences the stiffness and elastic properties of the NSs. Rossi et al. demonstrated in their study that the mechanical features of the NSs can be easily tuned by changing the molar ratio CD/cross-linker, on the other hand, the CD used for the synthesis does not affect the mechanical properties of the final NS [34, 49].
3.2.3 CD-based polyester NSs
Ester CD-based NSs are synthesized using dianhydrides or di/polycarboxylic acids, such as pyromellitic dianhydride (PMDA), ethylenediamine- tetraacetic dianhydride (EDTA dianhydride), butanetetracarboxylic dianhydride, citric acid [46, 50].
Dissimilarly from polycarbonate and polyurethane NSs, polyester NSs are generally able to absorb remarkable amounts of water (up to 25 times/g dry sample), and form stable hydrogels. Similarly as seen before with mechanical properties, the swelling capability of the CD-NSs is generally dependent on the degree of cross-linking. The swelling capability is usually inversely proportional to the density of cross-linking: the lower the degree of cross-linking, the higher the water uptake. The structure of the material dramatically influences chemical stability. Ester NSs are subjected to hydrolysis in aqueous media more easily than polycarbonate and polyurethane NSs. The structure is remarkably interesting because of the presence of free carboxyl groups in their chemical structure, moieties that can be exploited for the absorption of cations, using the material as an ionic exchange resin.
There are in literature many examples of the formation of complexes with a metal cation. The metal ions complexation ability of pyromellitic NSs is studied by Berto et al. in for different metal cations, such as Al3+, Mn2+, Co2+, Ni2+, Cu2+, Zn2+, Cd2+ and Pd2+.
In most cases, pyromellitic NSs were found to be capable of absorbing more than 70% of the tested cation .
A similar test of removing heavy metals from wastewaters, crosslinking also CDs with citric acid, is performed by Rubin Pedrazzo et al. in 2019 . At a metal concentration of 500 ppm, the pyromellitic NSs (substituted before absorption with Na+) exhibited a higher retention capacity than the citrate NSs. At lower metal concentrations (≤ 50 ppm) both the citrate and the pyromellitic NSs showed high retention capacities (up to 94% of the total amount of metal). While in the presence of interfering sea water salts, the citrate NSs were able to selectively adsorb a significantly higher amount of heavy metals than the pyromellitic NSs.
For ester NSs, similar studies of the correlation of cross-linking degree with properties are performed. Surprisingly, the highest cross-linking degree was observed in the sample prepared using the molar ratio 1: 6, CD: PMDA .
Higher contents of cross-linker, molar ratios like 1:8 and 1:10, led to a decrease of the degree of cross-linking; this is possibly related to the steric hindrance generated by the pyromellitic units linked to CDs. Interestingly, by working under limited dilution conditions during the reaction and with an even lower CD/cross-linker ratio (e.g., 1:2 molar ratio), it is possible to obtain a hyper-branched water-soluble polymer . As already described for carbonate NSs, Raman and Brillouin scattering experiments permitted Rossi et al. to evaluate a relationship between the mechanical characteristics of the polyester pyromellitic β-CD NS and the molar ratios CD/cross-linker: as seen before, stiffness and elasticity of the polymeric structure can be tuned by varying the amount of cross-linker .
4. Inclusion complex preparation and analysis
4.1 Preparation of inclusion complexes
Once the CD-NS is ready, the inclusion complex can be obtained by several procedures  as its summarized in Figure 2. Firstly, it is performed the classical mixing of drug and CD-NS in a solvent, commonly water for 24 h to form the complexes. In this procedure, we should consider the insoluble or soluble nature of our complexes. Depending on this, the desire fraction is purified. Using kneading, the drug and the CD-NS are mixed in a mortar with an appropriate quantity of water or another solvent to form the complexes. At this point, other additional techniques are used to form the powder: The solvent can be removed using lyophilization, co-evaporation, or spray-drying procedures.
4.2 Analysis of inclusion complexes
4.2.1 Ultraviolet/visible spectroscopy
UV–vis is a simple, easy, and fast method for studying the host-guest complexation when its formation changes any particularity of the spectrum of a guest molecule or to check the solubilization efficacy [14, 16, 58, 59].
4.2.2 Fourier-transform infra-red (FTIR)
This technique is usually used in solid complexes, generally in the range of 400–4000 cm−1, although it depends on the studied drug [58, 60]. Changes in the characteristics bands of the guest molecule or shifts in the wavenumber can indicate the formation of the complex. In addition, the same principle can be used to follow the CD-NS synthesis.
4.2.3 Nuclear magnetic resonance (NMR) spectroscopy
NMR is one of the most useful procedures to obtain complete analytical information of the CD-NS and the complex formed. An alteration in the chemical shift of the protons occurs when the drug enters the CD-NS providing specific information about the orientation of the guest molecule inside the cavity.
4.2.4 Thermogravimetric analysis (TGA)
TGA determines the changes of weight to temperature increases. The comparison of the weight loss profile of pure components, physical mixture, and the complex shows differences correlatives to the complex formation. A stage on TGA around 300°C is found in CD-NS due to CD decomposition .
4.2.5 Differential scanning calorimetry (DSC)
It can provide detailed information about their physical and energetic properties. The comparison of the thermal curves of single components, their physical mixture, and the presumed inclusion compound ought to provide insight into modifications and interactions due to the formation of the inclusion complex. The change that occurs in the fusion point of the guest molecule is usually hiding by the complex formation, while it remains in the physical mixture. This, and several modifications in the shape and temperature peak of the CD dehydration and/or with the disappearance of the drug melting peak among others, are proves of the complexation.
5. Applications in smart drug delivery
5.1 Improving solubility and controlled release of drugs
5.1.1 CD-based polyurethane NSs
Another study showed the capability of CD polyurethane to reduce the levels of natural product contaminants, particularly, Ochratoxin A (OTA) from spiked solutions between 1 and 10 μgL-1 . Following the attracted considerable interest that these polymers have shown in their use for water purification systems  and drug delivery , there were further done several chemical modifications on the CD NSs. Even though the modified CD NSs were used to enhance the properties and usefulness of CD NSs, their characterization at the molecular level remained a challenge. Therefore, a study described the structural characterization at the molecular level of both, native CD nanosponge polyurethanes and bionanosponge polyurethane cyclodextrin nanocomposite (pMWCNT-CD/Ag-TiO2) showing a great antibacterial and antifungal activity. The greatest antimicrobial activities were in the case of the developed polyurethane nanocomposite (pMWCNT-CD/Ag-TiO2). Consequently, it was concluded that this developed synthesis can be considered an active antimicrobial compound . Another potential application of CD polyurethane polymer is as immobilization supports in enzyme catalysis. The lipase was immobilized into the aforementioned polymers via physisorption. It is observed an improvement in the stability and catalytic activity of lipase, knowing that the enzymes are generally unstable, insoluble in organic solvents, and sensitive. Accordingly, this study presented the chance to prepare immobilized biocatalysts with tunable catalytic activities attributed to the alteration of reaction conditions . Further research was focused on the novel polyurethanes containing simultaneously β-cyclodextrin (β-CD), β-glycerophosphate groups, and hexamethylenediisocyanate (HDI). This polymer developed was used to complex the delivering therapeutic agents such as antibiotic ciprofloxacin. It was observed an improvement of the drug release in the case of the drug-polymers complexation than that of the free drug .
5.1.2 CD-based polycarbonate NSs
CD-based polycarbonate NSs synthesized using carbonyldiimidazole (CDI) showed antimicrobial activity against various microorganisms such as
5.1.3 CD-based polyester NSs
CD-based Ester NSs synthesized with pyromellitic dianhydride (PMDA) are well known for delivering, enhancing solubility, and preventing the degradation of various drugs such as Curcumin , Insulin , Resveratrol , Erlotinib hydrochloride , among others. Ethylenediaminetetraacetic dianhydride (EDTA) is another cross-linker to synthesize ester CD NSs. Based on HRMAS probe-heads in a high-resolution NMR spectrometer on the transport properties of Ibuprofen sodium salt (IP), it was found that these NSs can be utilized for the rational design of smart systems for drug delivery and controlled release . The various applications of CD-based polyester NSs ranging from the environment to pharmacy, chemistry, agriculture, gene delivery, cosmetics, biocatalysis, brought to a detailed study on their cross-linking density. Being a very challenging task, it presented the effect of cross-linking density on β-CD NSs physicochemical properties. Flory-Rehner theory and rheology enabled the authors to understand the correlation between the structural features of NSs and their physicochemical properties, which is a key requirement for future applications .
5.2 Last generations of NSs for selected target drug delivery
Stimuli-responsive NSs represent the third generation, polymers that have been designed to modulate their behavior according to the surrounding environment. In this case, changes in the chemical structure of the material were reported to be triggered by pH, temperature gradients, or oxidative/reducing conditions. This feature was exploited for studying the targeted release of drugs, changes in color, and permeability. The use of glutathione (GSH) bioresponsive CD-NS was proposed as the system to deliver anticancer drugs or bioactive compounds [114, 115, 116, 117]. This is because GSH is 100 to 1000 times higher inside cells than that in the extracellular fluids and circulation. Indeed, in cancer cells, this concentration is almost higher being a good system for target drug delivery . Different drugs such as doxorubicin  or bioactive compounds such as resveratrol  were tested showing a well-targeted drug delivery, and therefore is considered a promising therapy. In addition, the linkage of cholesterol was proposed as a good procedure for increase the targeted drug delivery of doxorubicin-loaded CD-NS .
Lastly, molecularly imprinted cyclodextrin-based polymers (Figure 3) define the fourth generation of NSs. Molecular imprinting represents a specific approach of inducing molecular recognition features to a three-dimensional polymer. This property can be achieved as a result of the presence of a template molecule introduced during synthesis. The template molecule after being removed from the polymer matrix leaves size-complementary vacancies, enabling the network to display high selectivity and affinity toward the chosen template. Eventually, molecularly imprinted CD-NSs are studied as suitable material to develop biosensors, drug delivery systems, catalysts, or synthetic antibody mimics [120, 121, 122]. A good example of this application is the L-Dopa as a novel possibility to treat Parkinson’s Disease. The molecularly imprinted CD-NSs showed a slower and more prolonged release profile than the non-imprinted NSs, indicating the good capacity to better complex L-Dopa than non-imprinted NS. The use of CDs in controlled and targeted drug delivery is shown in Table 2.
|Controlled Drug Delivery|
|CD-based Polyurethane NSs|
|Erythromycin, vancomycin, and rifampicin||βCD/HDI|||
|CD-based Polycarbonate NSs|
|Rilpivirine||βCD/CDI; PMDA; DPC||[90, 91]|
|CD-based Polyester NSs|
|Acetyl salicylic acid||βCD/PMDA|||
|Targeted Drug Delivery|
|DB103 - [2-(3, 4-dimethoxyphenyl)-3-phenyl-4H-pyrido]||βCD/DPC|||
|L-DOPA||βCD/CDI; PMDA (Molecularly imprinted cyclodextrin-based polymers)|||
|Doxorubicin||Tripeptide glutathione (GSH) nanosponge (NS)|||
|Erlotinib hydrochloride (ETB)||GSH-NS|||
CD-NSs are demonstrated to be safe, cheap, and biocompatible polymers. Consequently, several authors are focused on this field recently achieving novel applications. This chapter summarized the general information that will guide the advanced research to investigate the CD-NSs. Information about the routes of administration, synthesis protocols, recommendations, classifications, and applications of the novel synthesized materials, with special attention to targeted drug delivery, are mostly collected. It is shown the ability of CD-NSs to entrap drugs and to control their release from the matrix which can be modulated by different physicochemical agents.
As a remark, CD-NS is a good promise to improve the current problems in drug formulations and open novel strategies for drug delivery that identify the light in the future.
This work is the result of aid to postdoctoral training and improvement abroad (for Adrián Matencio, number 21229/PD/19) financed by the Fundación Séneca (Región de Murcia, Spain).
Conflict of interest
The authors declare no conflict of interest.